ИССЛЕДОВАНИЕ И РАЗРАБОТКА
ПОКРЫТИЙ ДЛЯ ЦИРКОНИЕВЫХ
Куприн А.С., Белоус В.А., Воеводин В.Н., Овчаренко В.Д.,
Василенко Р.Л., Зуёк В.А, Куштым Я.А., Толмачёва Г.Н.
Национальный научный центр «Харьковский физико-технический институт»,
г. Харьков, Украина
Improve the performance of zirconium alloys caused by:
Disability of serious consequences in case of accident and damage to the reactor
core (Fukushima-1; Zr + 2H2O = ZrO2 + 2H2), integrity of fuel rods under loss of
coolant accident (LOCA) type;
New generation LWR => Longer cycles, higher burn-up (>60 GWD/MTU)=> More
hard corrosive environment;
Fretting and debris damage of fuel claddings.
ATFC – Accident Tolerant Fuel Claddings for LWR
Two perspective ways to accident tolerant fuel claddings for LWR:
Long-term >10 years: new claddings (SiC/SiC composites, FeCrAl, Mo/FeCrAl etc.);
Medium term ≈10 years: current zirconium alloys with protective coatings (Cr, SiC,
The goal of ATF development is alternative fuel technologies for further enhance
safety and economics of commercial light water reactors.
High corrosion and radiation resistance at normal operation conditions;
Neutron economy (low cross section of thermal neutrons, the absence of long-lived
High thermal conductivity;
Barrier to hydrogen penetration ;
Improving mechanical properties of claddings;
Oxidation resistance in steam and air up to Т = 1200 °С;
Stability of functional properties at Т = 350…1200 °С
Requirements For Coatings On Zirconium Claddings:
Zirconium tubes (Zr1Nb alloy) with vacuum arc coatings based on chromium
A.S. Kuprin, V.А. Belous,V.N. Voyevodin,V.V. Bryk, R.L. Vasilenko,V.D. Ovcharenko, E.N. Reshetnyak, G.N. Tolmachova, P.N. V'yugov. Vacuum-arc chromium-
based coatings for protection of zirconium alloys from the high-temperature oxidation in air // Journal of Nuclear Materials 465 (2015) 400-406
Research and Development of Coatings for Advanced Zirconium
Nuclear Fuel Claddings
E110 (Zr1Nb) alloy is the main cladding material for WWER type reactors
Development of protective coatings for zirconium claddings in the world
Vacuum arc method for coatings deposition (KIPT)
Vacuum arc deposition method has advantages :
a wide range of metallic and ceramic coatings;
multi-layer, multi-component and nanostructured coatings;
a high degree of ionization(30-100%);
low deposition temperature (≤500 °C);
high deposition rate and high quality coatings (1-30 mkm/h).
Schematic diagram of the cathodic arc
Photo of plasma
stream from cathode
Structure analysis - SEM, ТEМ, XRD;
Concentration of elements – EDX, XRPA,
Mechanical characteristics of coatings and
surfaces – nanoindentation;
Mechanical characteristics of tubes – tensile
Saturation by hydrogen or deuterium from
the gas phase;
Corrosion – electrochemistry; autoclave;
thermocycling test in steam and air.
Methods of the investigations
Samples of Zr-1Nb claddings with coatings
TiAlN TiAlYN TiAlSiN
Samples of Zr-1Nb claddings : Ø -9.2 mm; wall thickness -0.7 mm; length -10 mm.
Oxidation resistant nitride and metallic vacuum arc coatings with thickness ~10 μm.
Chromium coatings on E110 alloy claddings
TEM image of coating structure and crystallites sizes
Photo of a tube fragment with Cr coating SEM image of coating cross section on tube
The chromium coating has a dense structure without pores and cracks
Crystallite size in the coating is near 500 nm
Anodic polarization curves for Zr-1Nb alloy
with coatings in the reactor water T=20 о
Nitride coatings increase the tensile strength σв
from 12 to 21% at 350 ° C.
Properties of the Zr1Nb claddings with coatings
Coating Zr1Nb Cr Cr/CrN TiN ZrN TiAlN TiAlYN TiAlSiN
H, GPa 2 5 25 30 28 32 34 36
Hardness of initial Zr1Nb alloy and vacuum arc coatings
Vacuum-arc nitride coatings increase the resistance of zirconium alloy to electrochemical corrosion in
Coatings have higher mechanical characteristics compared to uncoated zirconium alloys that should provide
a higher wear resistance of fuel cladding in normal in-reactor operating conditions.
Energy dependences of integral proton yields for Zr1% Nb with and without coatings saturated with deuterium at temperatures of
350, 450 and 550 °C for 2 hours.
500 600 700 800 900 1000
Al2O3 (2,5 mkm)
Al2O3 ( 8 mkm)
CrN (1,5 mkm)
Zr1Nb alloy with CrN, CrAl and Al2O3 coatings saturated with deuterium Р = 10-3
Pa, t= 120 min.
Depth distribution of implanted deuterium with energy 15 keV/D at 350 °С,
Zr1Nb Zr1Nb+CrN CrN, CrAl and Al2O3 coatings
serve as a barrier against the
penetration of deuterium
into zirconium in the
range from 350 to 550 °C.
Barrier properties of coatings against deuterium penetration
Depth, μm Depth, μm
E110 – 240 ppm Coated (14 μm)– 85 ppm
Resistance of E110 Alloy with Cr/CrN Coatings To Hydrogen Saturation
Coated (9 μm) – 100 ppm
Saturation of E110 alloy with Cr/CrN coatings by
hydrogen from the gas phase was carried out at a
temperature of 420 °C for 50 hours.
Cr/CrN coatings with thickness ~14 μm reduce the concentration of hydrogen in
zirconium alloy E110 from 240 to 85 ppm after the test in a hydrogen atmosphere.
Concentration of hydrides measured on the metallographic cross-sections of the
samples after tests using optical microscopy:
Cylindrical samples : Ø -9 mm, L – 10 mm;
Cr/CrN coatings with different thicknesses : 9 and
Oxidation of claddings with coatings in air at 750, 1000, 1100 °С
Weight gain of the samples after oxidation in air.
Coatings provide Zr-1Nb alloy protection from the oxidation in air for 1 h up to 1100 °С.
The best result demonstrates Cr coating.
Oxidation of Zr-1Nb with Cr coating in air at Т = 1100 °С, t= 1 h
High oxidation of the alloy E110 occurs to the depth of ~ 150 μm with formation
of a monoclinic cracking ZrO2 film;
Cr2O3 oxide film is formed up to the depth of 5 μm and the there is no phase
of ZrO2 in the chromium coating.
Thermocycling oxidation of coated claddings in steam at
Weight gain of samples after thermocyclic (3 times for
20 min) tests in the steam flow at 1020 °С
Only metallic coatings protect Zr1Nb after thermocyclic test
Oxidation of fuel rod models with coatings at 900 °C in steam
Fuel rod models, Ø - 9.1 mm; length - 80 mm;
internal pressure 1 atm.
With Cr coating
Ø 9,95 mm
Ø 9,6 mm
Fuel rod models with chromium coating (10 μm) demonstrate :
corrosion resistance in steam is 10 times better than without coating ;
lower increasing in tube diameter.
With Cr coating
Cyclic oxidation of fuel rod models with protective
coatings in steam
Thermal cycling tests of fuel claddings models with coatings in steam at T = 600 - 900 °C
- In the initial Zr1Nb cracking and delaminating of oxide after temperature cycling
testing observed ;
- Cr and Cr/CrN coatings demonstrate the best result without cracking and
Thermal cycling test: model fuel rods with internal pressure of 20 atm., holding for 1
min at test temperature, cooling to 100 °C; repeat 10 cycles at each temperature.
Autoclave tests of E110 model fuel rods with coatings, T=350 °C, pressurized
water P=150 atm., WWER water chemistry
Cr and Cr/CrN coatings demonstrate excellent corrosion resistance in
normal operation conditions
ATFC now is the one of the main safety task in reactor materials science;
Vacuum-arc nitride and metallic coatings were designed and tested on
zirconium fuel claddings in the concept of development ATFC in KIPT;
Coatings improve the mechanical properties (hardness and tensile
strength ) of zirconium tubes, increase the corrosion resistance and reduce
the amount of absorbed hydrogen;
Vacuum arc coatings reduce the oxidation rate of zirconium alloy under
high-temperature steam environment and in the air up to 1100 °C;
Zirconium claddings with chromium coatings showed the best resistance at
high temperature (600-1100 °C) tests;
Zirconium tubes with Cr and Cr/CrN coatings have high corrosion resistance
in nominal conditions and in the event of an accident.
1. A.S. Kuprin, V.А. Belous,V.N. Voyevodin,V.V. Bryk, R.L. Vasilenko,V.D. Ovcharenko, E.N. Reshetnyak, G.N.
Tolmachova, P.N. V'yugov. Vacuum-arc chromium-based coatings for protection of zirconium alloys from the
high-temperature oxidation in air // Journal of Nuclear Materials 465 (2015) 400-406
2. P.I. Stoev, V.A. Belous, V.N. Voyevodin, A.S. Kuprin, S.A. Leonov, V.D. Ovcharenko, M.A. Tikhonovsky, V.M.
Horoshih. Mechanical properties and acoustic parameters tubes of zirconium alloy Zr1%Nb with a protective
coatings // Problems Of Atomic Science And Technology 2015. №5(99), p. 87 – 97
3. I.E. Kopanetz, G.D. Tolstolutskaya, A.V. Nikitin, V.A. Bilous, A.S. Kuprin, V.D. Ovcharenko, R.L. Vasilenko. The
effect of Cr, Cr-N and Cr-Ox coatings on deuterium retention and penetration in zirconium alloy Zr-1Nb //
Problems Of Atomic Science And Technology 2015. №5(99), p. 81 -86
4. G.D. Tolstolutskaya, I.E. Kopanetz, V.V. Ruzhytskiy, V.A. Bilous, A.S. Kuprin, V.D. Ovcharenko, R.L. Vasilenko,
S.A. Leonov. Decrease of hydrogen saturation of zirconium alloys at modification of surface by complex ion-
plasma treatment // Problems Of Atomic Science And Technology 2015. №2(96), p. 119-123.
5. A.S. Kuprin, V.A. Belous, V.V. Bryk, R.L. Vasilenko, V.N. Voyevodin, V.D. Ovcharenko, G.N. Tolmachova, I.V.
Kolodiy, V.M. Lunyov, I.O. Klimenko. Vacuum-arc chromium coatings for Zr-1Nb alloy protection against high-
temperature oxidation in air // Problems Of Atomic Science And Technology 2015. №2 (96), p. 111-118.
6. A.S. Kuprin, V.A .Belous, V.N. Voyevodin, V.V. Bryk, R.L. Vasilenko, V.D. Ovcharenko, G.N. Tolmachova, P.N.
V’ygov. High-temperature air oxidation of E110 and Zr-1Nb alloys claddings with coatings // Problems Of
Atomic Science And Technology 2014. №1(89), p. 126-132
7. V.A. Belous, P.N. V´ygov, A.S. Kuprin, S.A. Leonov, G.I. Nosov, V.D. Ovcharenko, L.S. Ozhigov, A.G. Rudenko,
V.T. Savchenko, G.N. Tolmachеva, V.M. Khoroshikh. Mechanical characteristics of Zr1Nb alloy tube after
deposition of ion-plasma coatings // Problems Of Atomic Science And Technology 2013. №2(84), с. 140-143.
Thank for your attention!Thank for your attention!
KIPT is widely open for commonKIPT is widely open for common
research in ATFC area!research in ATFC area!